#------------------------------------------------------------------------------
#$Date: 2016-08-07 11:19:41 +0300 (Sun, 07 Aug 2016) $
#$Revision: 185214 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/22/51/7225180.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7225180
loop_
_publ_author_name
'Xue, Han'
'Zhang, Zhong'
'Pan, Rui'
'Yang, Bai-Feng'
'Liu, Hong-Sheng'
'Yang, Guo-Yu'
_publ_section_title
;
 Supramolecular nanotubes constructed from 3d--4f heterometallic
 sandwiched polyoxotungstate dimers
;
_journal_issue                   24
_journal_name_full               CrystEngComm
_journal_page_first              4643
_journal_paper_doi               10.1039/C6CE00755D
_journal_volume                  18
_journal_year                    2016
_chemical_formula_sum            'C12 H97 Fe2 N8 O105 P2 Sm W20'
_chemical_formula_weight         6034.97
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           165
_symmetry_cell_setting           trigonal
_symmetry_space_group_name_Hall  '-P 3 2"c'
_symmetry_space_group_name_H-M   'P -3 c 1'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_audit_update_record
;
2016-05-06 deposited with the CCDC.
2016-05-11 downloaded from the CCDC.
;
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            6
_cell_length_a                   31.9258(11)
_cell_length_b                   31.9258(11)
_cell_length_c                   20.7484(15)
_cell_measurement_reflns_used    3345
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      29.5267
_cell_measurement_theta_min      2.8262
_cell_volume                     18314.7(16)
_computing_cell_refinement       'Bruker FRAMBO'
_computing_data_collection       'Bruker FRAMBO'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.994
_diffrn_measured_fraction_theta_max 0.994
_diffrn_measurement_device_type  'multiwire proportional'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0000
_diffrn_reflns_av_sigmaI/netI    0.1596
_diffrn_reflns_limit_h_max       24
_diffrn_reflns_limit_h_min       -34
_diffrn_reflns_limit_k_max       39
_diffrn_reflns_limit_k_min       -35
_diffrn_reflns_limit_l_max       25
_diffrn_reflns_limit_l_min       -18
_diffrn_reflns_number            11942
_diffrn_reflns_theta_full        26.00
_diffrn_reflns_theta_max         26.00
_diffrn_reflns_theta_min         2.83
_diffrn_standards_decay_%        none
_diffrn_standards_interval_count none
_diffrn_standards_interval_time  none
_diffrn_standards_number         none
_exptl_absorpt_coefficient_mu    19.590
_exptl_absorpt_correction_T_max  0.6954
_exptl_absorpt_correction_T_min  0.2218
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            mossgreen
_exptl_crystal_density_diffrn    3.283
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       acicular
_exptl_crystal_F_000             16134
_exptl_crystal_size_max          0.11
_exptl_crystal_size_mid          0.06
_exptl_crystal_size_min          0.02
_platon_squeeze_details
;
;
_refine_diff_density_max         2.386
_refine_diff_density_min         -2.280
_refine_diff_density_rms         0.344
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.014
_refine_ls_matrix_type           full
_refine_ls_number_parameters     492
_refine_ls_number_reflns         11942
_refine_ls_number_restraints     40
_refine_ls_restrained_S_all      1.015
_refine_ls_R_factor_all          0.1255
_refine_ls_R_factor_gt           0.0729
_refine_ls_shift/su_max          0.012
_refine_ls_shift/su_mean         0.001
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0359P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1463
_refine_ls_wR_factor_ref         0.1572
_reflns_number_gt                5700
_reflns_number_total             11942
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c6ce00755d2.cif
_cod_data_source_block           x
_cod_depositor_comments
'Adding full bibliography for 7225178--7225181.cif.'
_cod_original_sg_symbol_H-M      P-3c1
_cod_database_code               7225180
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'y, x, -z+1/2'
'-x, -x+y, -z+1/2'
'x-y, -y, -z+1/2'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'-y, -x, z-1/2'
'x, x-y, z-1/2'
'-x+y, y, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
W1 W 0.35556(4) 0.33498(4) 0.08140(5) 0.0496(3) Uani 1 1 d .
W2 W 0.56577(4) 0.37971(4) 0.04471(5) 0.0544(3) Uani 1 1 d .
W3 W 0.51509(4) 0.38192(4) 0.27769(5) 0.0508(3) Uani 1 1 d .
W4 W 0.55418(4) 0.30838(4) 0.17602(6) 0.0585(3) Uani 1 1 d .
W5 W 0.34455(4) 0.26139(4) 0.22133(6) 0.0576(3) Uani 1 1 d .
W6 W 0.49421(4) 0.25559(4) 0.03513(6) 0.0659(3) Uani 1 1 d .
W7 W 0.44006(4) 0.24646(4) 0.26510(6) 0.0619(3) Uani 1 1 d .
W8 W 0.46236(4) 0.39206(4) -0.00497(5) 0.0514(3) Uani 1 1 d .
W9 W 0.37847(4) 0.19225(4) 0.12615(6) 0.0687(4) Uani 1 1 d .
W10 W 0.38941(4) 0.26834(4) -0.01608(6) 0.0633(3) Uani 1 1 d .
P1 P 0.45514(19) 0.32314(19) 0.1329(3) 0.0330(13) Uani 1 1 d .
Fe1 Fe 0.52304(10) 0.44218(10) 0.14771(14) 0.0371(7) Uani 1 1 d .
Sm1 Sm 0.40759(5) 0.40759(5) 0.2500 0.0461(4) Uani 1 2 d S
O1 O 0.5790(6) 0.5818(6) 0.1806(8) 0.071(5) Uani 1 1 d D
O2 O 0.5702(5) 0.5117(5) 0.1435(7) 0.057(4) Uani 1 1 d DU
O3 O 0.4822(5) 0.4611(5) 0.1900(6) 0.049(4) Uani 1 1 d D
O4 O 0.4703(5) 0.3949(6) 0.3010(8) 0.065(5) Uani 1 1 d .
O5 O 0.3754(5) 0.3207(5) 0.2524(8) 0.063(5) Uani 1 1 d .
O6 O 0.3859(5) 0.3781(5) 0.1426(7) 0.048(4) Uani 1 1 d .
O7 O 0.5517(5) 0.4361(5) 0.2280(7) 0.044(4) Uani 1 1 d .
O8 O 0.5500(6) 0.3940(6) 0.3466(8) 0.077(6) Uani 1 1 d .
O9 O 0.4873(5) 0.4297(5) 0.0648(6) 0.056(4) Uani 1 1 d .
O10 O 0.5667(5) 0.4248(5) 0.1003(7) 0.049(4) Uani 1 1 d U
O11 O 0.5518(5) 0.3532(6) 0.2272(8) 0.062(5) Uani 1 1 d .
O12 O 0.4712(6) 0.3106(6) 0.2918(7) 0.058(4) Uani 1 1 d .
O13 O 0.5988(6) 0.3012(6) 0.2136(8) 0.069(5) Uani 1 1 d .
O14 O 0.5949(5) 0.3576(5) 0.1125(9) 0.069(5) Uani 1 1 d .
O15 O 0.6153(5) 0.4138(6) -0.0011(7) 0.062(5) Uani 1 1 d .
O16 O 0.5140(5) 0.3774(5) -0.0083(7) 0.053(4) Uani 1 1 d .
O17 O 0.4800(6) 0.4342(5) -0.0673(7) 0.063(5) Uani 1 1 d .
O18 O 0.3981(5) 0.3820(5) 0.0147(6) 0.046(4) Uani 1 1 d .
O19 O 0.3017(7) 0.3355(6) 0.0665(10) 0.092(6) Uani 1 1 d .
O20 O 0.3306(5) 0.2795(4) 0.1356(6) 0.043(4) Uani 1 1 d .
O21 O 0.2856(6) 0.2321(7) 0.2527(9) 0.093(6) Uani 1 1 d .
O22 O 0.3782(7) 0.2393(6) 0.2828(9) 0.083(6) Uani 1 1 d .
O23 O 0.4443(7) 0.2169(6) 0.3310(9) 0.088(6) Uani 1 1 d U
O24 O 0.4987(5) 0.2593(5) 0.2165(7) 0.048(4) Uani 1 1 d .
O25 O 0.5356(6) 0.2619(6) 0.1039(9) 0.075(5) Uani 1 1 d .
O26 O 0.5440(5) 0.3166(5) 0.0030(7) 0.053(4) Uani 1 1 d .
O27 O 0.4281(6) 0.3308(6) -0.0567(7) 0.066(5) Uani 1 1 d .
O28 O 0.3452(5) 0.2843(5) 0.0122(8) 0.060(5) Uani 1 1 d .
O29 O 0.3313(6) 0.2006(7) 0.1713(8) 0.084(6) Uani 1 1 d .
O30 O 0.4068(5) 0.1903(5) 0.2079(8) 0.066(5) Uani 1 1 d .
O31 O 0.4396(6) 0.2113(6) 0.0894(8) 0.067(5) Uani 1 1 d .
O32 O 0.4500(5) 0.2659(5) -0.0108(7) 0.049(4) Uani 1 1 d .
O33 O 0.3703(7) 0.2218(7) 0.0483(11) 0.099(7) Uani 1 1 d .
O34 O 0.4981(6) 0.2135(6) -0.0122(9) 0.082(6) Uani 1 1 d .
O35 O 0.3462(6) 0.1297(6) 0.1058(11) 0.098(7) Uani 1 1 d .
O36 O 0.3615(7) 0.2304(7) -0.0832(9) 0.090(6) Uani 1 1 d .
O37 O 0.4757(5) 0.3673(5) 0.1755(7) 0.049(4) Uani 1 1 d U
O38 O 0.4217(5) 0.2768(5) 0.1666(7) 0.056(4) Uani 1 1 d .
O39 O 0.4989(5) 0.3188(5) 0.1072(7) 0.051(4) Uani 1 1 d .
O40 O 0.4264(5) 0.3268(5) 0.0757(7) 0.051(4) Uani 1 1 d .
C1 C 0.5575(8) 0.5366(8) 0.1751(13) 0.088(9) Uani 1 1 d DU
C2 C 0.5096(7) 0.5098(6) 0.2118(9) 0.047(6) Uani 1 1 d DU
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Fe Fe 0.3463 0.8444 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sm Sm -0.1638 3.4418 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O19 W1 O6 106.1(7) . .
O19 W1 O20 99.0(8) . .
O6 W1 O20 96.4(6) . .
O19 W1 O18 99.9(8) . .
O6 W1 O18 90.6(6) . .
O20 W1 O18 157.1(5) . .
O19 W1 O28 96.4(7) . .
O6 W1 O28 157.4(6) . .
O20 W1 O28 81.5(6) . .
O18 W1 O28 83.6(6) . .
O19 W1 O40 166.2(7) . .
O6 W1 O40 86.6(6) . .
O20 W1 O40 84.7(5) . .
O18 W1 O40 74.0(5) . .
O28 W1 O40 70.8(5) . .
O15 W2 O10 101.8(7) . .
O15 W2 O16 102.1(7) . .
O10 W2 O16 93.7(6) . .
O15 W2 O26 98.5(7) . .
O10 W2 O26 159.6(6) . .
O16 W2 O26 81.7(6) . .
O15 W2 O14 99.9(7) . .
O10 W2 O14 90.4(7) . .
O16 W2 O14 156.3(6) . .
O26 W2 O14 86.4(6) . .
O15 W2 O39 168.9(6) . .
O10 W2 O39 87.4(5) . .
O16 W2 O39 83.2(5) . .
O26 W2 O39 72.4(5) . .
O14 W2 O39 73.7(5) . .
O8 W3 O4 103.4(8) . .
O8 W3 O7 102.5(8) . .
O4 W3 O7 98.2(7) . .
O8 W3 O12 98.0(8) . .
O4 W3 O12 92.2(7) . .
O7 W3 O12 154.1(6) . .
O8 W3 O11 94.1(7) . .
O4 W3 O11 161.3(7) . .
O7 W3 O11 84.3(6) . .
O12 W3 O11 78.6(6) . .
O8 W3 O37 173.0(7) . .
O4 W3 O37 83.0(7) . .
O7 W3 O37 73.3(5) . .
O12 W3 O37 84.7(5) . .
O11 W3 O37 80.0(5) . .
O13 W4 O11 101.7(7) . .
O13 W4 O24 100.6(7) . .
O11 W4 O24 90.1(6) . .
O13 W4 O14 98.5(7) . .
O11 W4 O14 91.9(7) . .
O24 W4 O14 160.0(6) . .
O13 W4 O25 101.4(7) . .
O11 W4 O25 156.9(6) . .
O24 W4 O25 84.8(7) . .
O14 W4 O25 85.6(7) . .
O13 W4 O39 170.5(7) . .
O11 W4 O39 85.1(6) . .
O24 W4 O39 86.0(5) . .
O14 W4 O39 74.4(6) . .
O25 W4 O39 72.0(5) . .
O21 W5 O5 108.1(8) . .
O21 W5 O20 98.7(8) . .
O5 W5 O20 95.8(7) . .
O21 W5 O22 101.3(8) . .
O5 W5 O22 92.1(8) . .
O20 W5 O22 155.1(6) . .
O21 W5 O29 91.4(8) . .
O5 W5 O29 160.5(7) . .
O20 W5 O29 81.5(7) . .
O22 W5 O29 83.3(8) . .
O21 W5 O38 162.0(7) . .
O5 W5 O38 89.4(6) . .
O20 W5 O38 83.1(5) . .
O22 W5 O38 73.4(6) . .
O29 W5 O38 71.1(6) . .
O34 W6 O32 101.8(8) . .
O34 W6 O25 101.2(9) . .
O32 W6 O25 156.9(7) . .
O34 W6 O26 104.4(6) . .
O32 W6 O26 87.6(6) . .
O25 W6 O26 88.5(6) . .
O34 W6 O31 98.6(7) . .
O32 W6 O31 86.7(6) . .
O25 W6 O31 88.0(7) . .
O26 W6 O31 157.0(6) . .
O34 W6 O39 172.9(7) . .
O32 W6 O39 84.6(5) . .
O25 W6 O39 72.5(6) . .
O26 W6 O39 72.4(5) . .
O31 W6 O39 84.8(6) . .
O23 W7 O12 102.9(8) . .
O23 W7 O22 98.3(9) . .
O12 W7 O22 91.5(7) . .
O23 W7 O30 97.8(8) . .
O12 W7 O30 159.1(7) . .
O22 W7 O30 87.3(7) . .
O23 W7 O24 101.2(8) . .
O12 W7 O24 89.7(6) . .
O22 W7 O24 159.7(7) . .
O30 W7 O24 84.5(6) . .
O23 W7 O38 170.7(8) . .
O12 W7 O38 85.1(6) . .
O22 W7 O38 76.7(6) . .
O30 W7 O38 74.3(6) . .
O24 W7 O38 83.2(5) . .
O17 W8 O9 102.6(7) . .
O17 W8 O16 100.1(7) . .
O9 W8 O16 92.5(7) . .
O17 W8 O18 100.9(7) . .
O9 W8 O18 91.2(6) . .
O16 W8 O18 157.3(6) . .
O17 W8 O27 99.4(7) . .
O9 W8 O27 157.9(6) . .
O16 W8 O27 81.9(7) . .
O18 W8 O27 86.3(6) . .
O17 W8 O40 172.1(7) . .
O9 W8 O40 83.1(6) . .
O16 W8 O40 85.0(6) . .
O18 W8 O40 73.3(5) . .
O27 W8 O40 75.1(6) . .
O35 W9 O31 101.0(8) . .
O35 W9 O29 102.6(8) . .
O31 W9 O29 156.4(7) . .
O35 W9 O30 100.9(8) . .
O31 W9 O30 86.5(7) . .
O29 W9 O30 89.4(8) . .
O35 W9 O33 101.8(9) . .
O31 W9 O33 82.9(7) . .
O29 W9 O33 91.9(8) . .
O30 W9 O33 156.4(7) . .
O35 W9 O38 174.0(8) . .
O31 W9 O38 82.2(6) . .
O29 W9 O38 74.4(6) . .
O30 W9 O38 74.0(6) . .
O33 W9 O38 83.7(6) . .
O36 W10 O28 104.5(7) . .
O36 W10 O33 99.6(8) . .
O28 W10 O33 90.1(8) . .
O36 W10 O27 101.9(8) . .
O28 W10 O27 92.1(7) . .
O33 W10 O27 157.0(7) . .
O36 W10 O32 100.6(7) . .
O28 W10 O32 154.6(6) . .
O33 W10 O32 82.2(7) . .
O27 W10 O32 86.1(7) . .
O36 W10 O40 175.2(7) . .
O28 W10 O40 72.0(5) . .
O33 W10 O40 83.9(6) . .
O27 W10 O40 75.2(5) . .
O32 W10 O40 83.1(5) . .
O38 P1 O37 114.4(9) . .
O38 P1 O40 106.1(9) . .
O37 P1 O40 112.2(8) . .
O38 P1 O39 107.4(8) . .
O37 P1 O39 107.0(8) . .
O40 P1 O39 109.6(8) . .
O3 Fe1 O7 93.9(6) . .
O3 Fe1 O2 85.4(6) . .
O7 Fe1 O2 91.0(6) . .
O3 Fe1 O9 92.7(7) . .
O7 Fe1 O9 164.8(6) . .
O2 Fe1 O9 103.1(6) . .
O3 Fe1 O10 177.3(6) . .
O7 Fe1 O10 88.0(6) . .
O2 Fe1 O10 92.6(6) . .
O9 Fe1 O10 85.9(6) . .
O3 Fe1 O37 91.0(6) . .
O7 Fe1 O37 76.6(6) . .
O2 Fe1 O37 166.8(6) . .
O9 Fe1 O37 89.7(6) . .
O10 Fe1 O37 91.3(6) . .
O6 Sm1 O6 139.9(6) . 4
O6 Sm1 O5 76.6(5) . 4
O6 Sm1 O5 72.2(5) 4 4
O6 Sm1 O5 72.2(5) . .
O6 Sm1 O5 76.6(5) 4 .
O5 Sm1 O5 77.0(7) 4 .
O6 Sm1 O3 141.1(5) . 4
O6 Sm1 O3 77.9(5) 4 4
O5 Sm1 O3 120.9(5) 4 4
O5 Sm1 O3 141.8(5) . 4
O6 Sm1 O3 77.9(5) . .
O6 Sm1 O3 141.1(5) 4 .
O5 Sm1 O3 141.8(5) 4 .
O5 Sm1 O3 120.9(5) . .
O3 Sm1 O3 67.8(6) 4 .
O6 Sm1 O4 77.7(5) . 4
O6 Sm1 O4 115.8(5) 4 4
O5 Sm1 O4 73.7(5) 4 4
O5 Sm1 O4 141.9(5) . 4
O3 Sm1 O4 75.5(5) 4 4
O3 Sm1 O4 73.4(5) . 4
O6 Sm1 O4 115.8(5) . .
O6 Sm1 O4 77.7(5) 4 .
O5 Sm1 O4 141.9(5) 4 .
O5 Sm1 O4 73.7(5) . .
O3 Sm1 O4 73.4(5) 4 .
O3 Sm1 O4 75.5(5) . .
O4 Sm1 O4 142.3(7) 4 .
C1 O2 Fe1 112.9(14) . .
C2 O3 Fe1 110.4(12) . .
C2 O3 Sm1 116.7(10) . .
Fe1 O3 Sm1 126.2(6) . .
W3 O4 Sm1 138.4(9) . .
W5 O5 Sm1 155.4(10) . .
W1 O6 Sm1 156.8(8) . .
W3 O7 Fe1 117.4(7) . .
W8 O9 Fe1 148.2(10) . .
W2 O10 Fe1 142.0(8) . .
W4 O11 W3 153.1(9) . .
W7 O12 W3 152.9(9) . .
W4 O14 W2 121.1(7) . .
W8 O16 W2 141.3(7) . .
W8 O18 W1 122.2(7) . .
W1 O20 W5 138.5(8) . .
W7 O22 W5 122.6(9) . .
W4 O24 W7 143.2(8) . .
W6 O25 W4 125.7(8) . .
W6 O26 W2 125.1(7) . .
W10 O27 W8 121.8(8) . .
W10 O28 W1 127.0(7) . .
W9 O29 W5 125.4(9) . .
W9 O30 W7 123.2(7) . .
W9 O31 W6 150.0(7) . .
W6 O32 W10 151.4(8) . .
W10 O33 W9 155.6(10) . .
P1 O37 Fe1 127.7(9) . .
P1 O37 W3 130.0(8) . .
Fe1 O37 W3 90.7(5) . .
P1 O38 W7 125.8(9) . .
P1 O38 W9 130.6(9) . .
W7 O38 W9 88.0(5) . .
P1 O38 W5 123.2(8) . .
W7 O38 W5 87.2(5) . .
W9 O38 W5 89.0(5) . .
P1 O39 W4 123.8(8) . .
P1 O39 W2 125.4(8) . .
W4 O39 W2 90.9(5) . .
P1 O39 W6 126.2(8) . .
W4 O39 W6 89.7(4) . .
W2 O39 W6 90.0(4) . .
P1 O40 W1 126.7(8) . .
P1 O40 W8 123.0(8) . .
W1 O40 W8 90.4(4) . .
P1 O40 W10 127.3(8) . .
W1 O40 W10 90.0(5) . .
W8 O40 W10 87.7(4) . .
O2 C1 O1 128(2) . .
O2 C1 C2 117.3(19) . .
O1 C1 C2 114.6(18) . .
O3 C2 C1 110.4(15) . .
O3 C2 C2 108.4(12) . 4
C1 C2 C2 119.7(16) . 4
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
W1 O19 1.754(18) .
W1 O6 1.764(13) .
W1 O20 1.904(12) .
W1 O18 1.993(14) .
W1 O28 2.063(14) .
W1 O40 2.406(15) .
W2 O15 1.693(13) .
W2 O10 1.832(13) .
W2 O16 1.957(15) .
W2 O26 1.972(14) .
W2 O14 1.999(17) .
W2 O39 2.423(14) .
W3 O8 1.733(14) .
W3 O4 1.742(14) .
W3 O7 1.844(14) .
W3 O12 2.010(16) .
W3 O11 2.094(15) .
W3 O37 2.389(15) .
W4 O13 1.737(16) .
W4 O11 1.814(16) .
W4 O24 1.876(13) .
W4 O14 1.963(16) .
W4 O25 1.977(19) .
W4 O39 2.420(15) .
W5 O21 1.754(17) .
W5 O5 1.764(14) .
W5 O20 1.988(14) .
W5 O22 2.009(18) .
W5 O29 2.052(17) .
W5 O38 2.527(14) .
W6 O34 1.718(15) .
W6 O32 1.865(15) .
W6 O25 1.887(17) .
W6 O26 1.916(15) .
W6 O31 1.960(16) .
W6 O39 2.457(13) .
W7 O23 1.705(15) .
W7 O12 1.859(15) .
W7 O22 1.907(18) .
W7 O30 1.961(16) .
W7 O24 1.981(14) .
W7 O38 2.456(15) .
W8 O17 1.744(15) .
W8 O9 1.794(15) .
W8 O16 1.926(13) .
W8 O18 1.954(13) .
W8 O27 2.008(15) .
W8 O40 2.464(13) .
W9 O35 1.781(16) .
W9 O31 1.891(15) .
W9 O29 1.901(16) .
W9 O30 1.938(16) .
W9 O33 1.95(2) .
W9 O38 2.484(16) .
W10 O36 1.767(17) .
W10 O28 1.820(15) .
W10 O33 1.86(2) .
W10 O27 1.937(16) .
W10 O32 1.976(14) .
W10 O40 2.510(15) .
P1 O38 1.496(15) .
P1 O37 1.509(14) .
P1 O40 1.540(14) .
P1 O39 1.563(13) .
Fe1 O3 1.904(13) .
Fe1 O7 1.957(14) .
Fe1 O2 1.965(15) .
Fe1 O9 1.990(14) .
Fe1 O10 1.999(13) .
Fe1 O37 2.171(13) .
Sm1 O6 2.383(13) .
Sm1 O6 2.383(13) 4
Sm1 O5 2.428(15) 4
Sm1 O5 2.428(15) .
Sm1 O3 2.464(14) 4
Sm1 O3 2.464(14) .
Sm1 O4 2.472(15) 4
Sm1 O4 2.472(15) .
O1 C1 1.256(16) .
O2 C1 1.243(16) .
O3 C2 1.424(16) .
C1 C2 1.530(17) .
C2 C2 1.58(4) 4
loop_
_platon_squeeze_void_nr
_platon_squeeze_void_average_x
_platon_squeeze_void_average_y
_platon_squeeze_void_average_z
_platon_squeeze_void_volume
_platon_squeeze_void_count_electrons
_platon_squeeze_void_content
1 -0.005 -0.004 -0.004 9473 6804 ' '
